{'fraction_non_alphanumeric': 0.03201512333445132, 'fraction_numerical': 0.019087111626063358, 'mean_word_length': 4.461781848459617, 'pattern_counts': {'":': 0, '<': 2, '<?xml version=': 0, '>': 1, 'https://': 0, 'lorem ipsum': 0, 'www.': 8, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
Nanoslot metasurface design and characterization for enhanced organic light-emitting diodes

We investigate bottom-emitting organic light-emitting diodes (B-OLEDs) integrated with metasurface (MS) to analyze the effect of the structural parameters on the output performance. The performance of the MS-integrated B-OLED (MIB-OLED) is evaluated by out-coupling efficiency (OCE) and reflection of the ambient light, while attention is paid mainly to dielectric capping and metal structure of MS that may influence excitation of surface plasmon (SP). The results suggest that layer thicknesses affect the performance by as much as 10% for the OCE and up to 32% for reflectance. The OCE is in general weakly affected by the structural parameters of MS. In contrast, the reflectance characteristics are found to be dominated by localized SP that is largely determined by the length and the width of a unit slot of MS. An optimization factor introduced to evaluate the performance based on out-coupling power to the radiation mode and reflectance of MIB-OLEDs confirms that integration with MS improves performance by 16% over conventional planar structure. In particular, MIB-OLED is found to enhance OCE by 51% with Lambertian-like pattern. Enhanced performance is experimentally confirmed. The findings provide insights on how to optimize the MS structure to produce MIB-OLEDs with enhanced out-coupled power and contrast ratio.

where V(λ) represents the eye sensitivity spectrum. R(λ) is the reflectance at the OLED surface and S(λ) an optical spectrum of ambient light. Equation (1) implies that reduced R D would increase contrast. Reflectance R D of external light may also affect contrast of an image. Therefore, both CR and R D are important in OLEDs. In order to diminish the reflection of the ambient light, a circular polarizer composed of a quarter-wavelength plate and a linear polarizer has been often adopted in OLEDs 10,11 . Although a circular polarizer can keep the reflection of ambient light under 4-6%, it may increase panel thickness thus reduce flexibility and inevitable power absorption losses bring about more than 50% cutback of the out-coupling efficiency (OCE) 9 , which represents the efficiency of extracting photons out of the cavity and is expressed as a ratio of external quantum efficiency (EQE) to internal quantum efficiency (IQE), i.e., OCE = EQE/IQE. The MS is based on conventional visible range perfect absorber and consists of a periodic array of unit cells, which is shown enlarged in the inset: with multiple slots for the MS, the design may take advantage of many design parameters to optimize LSP absorption spectrum. The MS to absorb ambient light was assumed on a glass substrate, above which transparent anode of indium tin oxide (ITO) and a thin dielectric layer, called a capping layer (CPL), are stacked. The CPL is used as an optical functional layer to optimize the OCE or tune the spectral distributions 49 . The unit MS cell is a gold layer with eight cut-out slots filled with a dielectric material (n = 1.7), which is the same as the material of the CPL. Two cut-out slots with an identical width of W and different lengths of L 1 and L 2 are combined together in quadrant sections rotated orthogonally. The period of the unit MS is fixed at Λ = 500 nm. For comparison of the optical performances, we have calculated wavelength-dependent spectra and OCE.
The layer cross-section of a MIB-OLED is illustrated in Fig. 1b, which also shows the cross-section of a conventional planar B-OLED structure. The planar B-OLED uses 100-nm aluminum as a top cathode, 15-nm calcium as an electron injecting layer (EIL), 130-nm tris-(8-hydroxyquinoline) aluminum (Alq 3 ) as both the electron-transport layer (ETL) and emission layer (EML), 20-nm poly (3,4)-ethylendioxythiophene doped with poly(styrene sulfonate) (PEDOT:PSS) as a hole injection layer (HIL), 50-nm thick ITO as a bottom anode, 1,1-bis[(di-4-tolylamino)phenyl]cyclohexane (TAPC) as a dielectric CPL (thickness: x nm) on a thick glass substrate, as shown in Fig. 1b. The refractive indices of the materials used in the B-OLED model were obtained by ellipsometry or taken from the literature 50,51 . For the OCE, simulation was performed at the wavelength of 520 nm which coincides with the photoluminescence peak of Alq 3 52 . A dipole emitter is isotropic and 50 nm apart from the Ca layer (EIL) having a δ-distributed emission zone based on two-beam interference of microcavity effects for the radiation mode. The thicknesses of ETL and EML were determined to optimize the OCE in the vicinity of λ = 520 nm so as to maximize multiple-beam interference due to micro-cavity effects. For the MIB-OLED model, a mixed-slot layer was added below CPL (height: y nm). The coupling-power to radiation, substrate, and waveguide (WG) modes were calculated by surface integration of amplitudes of Poynting vectors in the domain relevant to each mode, as shown in Fig. 1c-e. The plasmon mode and absorption losses were calculated by volume integration of power dissipation in the whole OLED device, as shown in Fig. 1f.
The MIB-OLED model is designed to consider the interaction between the top cathode (aluminum) and the bottom gold MS for leading to improved absorption. The top cathode layer plays the role of an optical mirror to reflect incident light, while the bottom MS acts as a scatterer causing excitation of surface plasmon (SP) modes. Two crucial mechanisms that may be involved in resonant transmission are known to be the excitation of SPP and LSP 53,54 . The formation of SPP modes is attributed to the interference of multiple waves scattered by slot arrays and depends on the arrangement and thickness of organic and dielectric layers. LSP resonance (LSPR) is also affected by the shape and the size of the unit slot because LSP modes are generated at the edges of the slot.
The optical properties of MIB-OLEDs were analyzed based on the OCE and the luminous reflectance. IQE of fluorescent OLEDs limited to 25% due to the use of singlet excitons in the cavity affects the OCE little. To www.nature.com/scientificreports/ increase the CR of OLEDs, the reflectance from the ambient light should be diminished. On the other hand, the emitted light from dipole emitters needs to be efficiently out-coupled to the radiation mode to achieve high power efficiency. To achieve an optimum with this consideration, we set two groups of geometrical parameters for the MS. The first group of parameters concerns the thickness of CPL (d CPL ) and the gold MS layer (d MS ) that are associated primarily with the resonance between the top metal and the bottom gold layer. The other group is the one consisting of the length of the shorter slot (L 2 ) and the slot width (W) in connection with the effect of localized fields.
Numerical method. For the 3D calculation in the far-field, finite element method (FEM) was used under appropriate boundary conditions [55][56][57] . FEM has been used to calculate electromagnetic properties of an optical structure in many studies for the broad applicability and robustness in modeling and is often preferred over other techniques such as finite difference time domain (FDTD) and discontinuous galerkin time-domain (DGTD) method because it employs flexible mesh structure with reduced time load. We have used a commercial software COMSOL Multiphysics with its wave optics module in which Maxwell equations are numerically solved in small meshes that divide calculation domains. In the calculation of the OCE, a scattering boundary condition was used at all the outer boundaries of the 3D OLED device to eliminate reflection at the outer boundary. Although a pixel of OLEDs has a size on the order of tens of micrometers, a square pixel was assumed here to be 2 μm × 2 μm in the lateral plane in order to minimize workstation memory usage. The light emission from exciton in the EML is modeled as the radiation of a Hertzian point dipole 58 .
Because plasmonic absorption may increase temperature of OLEDs thus decrease the device lifetime, we have also analyzed thermal property of MIB-OLED using wave-coupled heat transfer equation 59 . The power dissipation calculated in the optical model was replaced as the heat source term in the heat transfer equation. Wave-coupled time-dependent heat transfer equation was then solved by FEM to obtain the temperature distribution in the OLED model. Amplitude of the dipole moment was matched to the emitted normal power intensity at 30 mW/cm 2 with B-OLEDs 60 . For thermal analysis, we used properties of organic materials reported in the past [61][62][63] . With external ambient temperature set to be T amb = 293.15 K (room temperature), the local temperature www.nature.com/scientificreports/ of MIB-OLED was found to rise up to T max = 293.18 K, i.e., the rise of temperature poses an insignificant effect so as to change the lifetime of OLEDs.
In the calculation of reflectance, periodic structure was modeled with periodic boundary conditions at the outermost side boundaries. Port boundary conditions were used at the lowermost boundary of the ambience and at the uppermost of the cathode to model plane waves from an ambient region with normal incidence to the device. Because thick glass substrate acts as an incoherent layer, coherent calculation results were averaged using the equispaced thickness method (ETM) with three additional thicknesses of the glass substrate: where λ is the wavelength of the incident ambient light and n g is the refractive index of the glass substrate. The averaged electric field intensity considering incoherency was obtained by where E(x, y, z, d j ) represents the electric field obtained by the coherent calculation at the x, y, and z position of the B-OLED structure in the Cartesian coordinates with the j-th thickness of glass substrate using FEM (j = 1, 2, 3). Using the calculated electric field intensities, the spatial distribution of light absorption can be obtained. The total reflectance of the B-OLED considering incoherency of the glass substrate can then be easily calculated by R tot = 1 − A, where A represents the absorbance of the whole device, because the top metal cathode suppresses light transmission through the cathode. The accuracy of the ETM was demonstrated in previous studies 64,65 . The reflectance of thin-film organic solar cells calculated by the ETM with three additional incoherent layers shows that the deviation from the exact solution can be maintained under 2% 64 . Although averaging over a larger number of incoherent layers may enhance the accuracy of the results, we used three incoherent layers to reduce the calculation time. To calculate the luminous reflectance R D , D65 (a standard light source) was chosen to be the ambient light source. The accuracy of FEM is affected by the mesh size, i.e., with a reduced mesh size, accuracy is improved at the expense of long calculation time and more computational resource. We set the maximum mesh size to be 60 nm to optimize calculation time and accuracy. Out-coupling efficiency. d CPL and d MS were varied to understand the resonance effect of the meta-structure on the out-coupling mechanism. The out-coupling ratios of MIB-OLEDs with respect to d CPL and d MS are presented in Fig. 2a. The MS composed of two slots has different lengths of L 1 = 240 nm and L 2 = 160 nm. The width of a unit slot W is set to 110 nm. d CPL and d MS were varied from 20 to 100 nm in a step of 10 nm. The CPL is assumed to be a non-absorbing dielectric layer sandwiched between top and bottom metal layers.

Results and discussion
Change in d CPL may cause multiple resonances inside the OLED cavity due to the redistribution of photonic density of states in the quantum mechanical approach 53,66 . Because multiple interferences are governed by the thickness of the dielectric layer between top and bottom metal, an increased thickness leads to the fluctuation in the OCE. In Fig. 2a, d CPL increases the OCE up to d CPL = 50 nm, after which the OCE is reduced regardless of d MS even as the CPL becomes thicker. This is because d CPL = 50 nm satisfies the condition of constructive interference. Interestingly, even though the highest out-coupling power ratio from the whole emission power is obtained at d CPL = 50 nm, higher power flow to the air mode can be achieved with d CPL = 60 nm. The parameter set that leads to an optimum for the OCE and the power flow into the air mode can be disparate, which is why the whole coupling power to the multiple modes is varied by the way that a dipole emitter is configured, e.g., under resonant cavity condition.
On the other hand, the OCE is decreased as d MS increases. High extinction of gold makes MS actively absorb emitted light from the emission layer in thick MS. When d MS increases from 20 to 100 nm, therefore, the OCE falls dramatically below half. Here, we have required d MS ≥ 20 nm because light absorption of ambience through MS is essential to reduce background noise. In the case of d CPL = 60 nm and d MS = 20 nm, the OCE reaches a maximum at 15.9%. In contrast, the minimum OCE was obtained as 6.0% with d CPL = 100 nm and d MS = 100 nm.
Reflection characteristics. To enhance the CR of OLEDs, reflection caused by the ambient light at the bottom glass surface should be minimized. The mixed slots tend to act as a perfect absorber of light ambience in the visible wavelength range. Like the case of the OCE, two different lengths of the unit slot L 1 and L 2 are fixed at L 1 = 240 nm and L 2 = 160 nm. The slot width W is selected to be 110 nm. The reflectance of light ambience, when the light is incident along the normal direction toward the glass substrate, was calculated varying d CPL and d MS . The range was set equally to the out-coupling calculation between 20 and 100 nm in a step of 10 nm. Calculation of reflectance was performed in the wavelength range from λ 1 = 400 to λ 2 = 700 nm and converted to the luminous reflectance R D using Eq. (2). www.nature.com/scientificreports/ Figure 2a shows the luminous reflectance varying d CPL and d MS . Most notably, thicker MS reduces reflectance regardless of d CPL . Obviously, a thick MS layer of gold increases absorption of light emitted from a dipole emitter and of external light ambience. The reflectance is also reduced when SPP waves are excited. Because the reflectance characteristics are associated with the interaction between top cathode and bottom MS layers, the thickness of MS may affect the dielectric layer thickness conditioned for efficient SPP excitation, e.g., with d MS = 20 nm, the luminous reflectance (R D ) becomes the lowest at R D = 29.0% at d CPL = 20 nm. When d MS > 60 nm, d CPL corresponding to the minimum R D is switched from 20 to 90 or 100 nm. Note that R D is dominated by the characteristics in the wavelength range of 500-600 nm, in which thicker MS changes the dielectric layer thickness to maximize absorption caused by the SP mode, related to spectra of eye sensitivity and ambient light. Overall, the minimum reflectance was obtained as 13.9% at d CPL = 90 nm and d MS = 100 nm. The maximum luminous reflectance was found to reach up to 46.2% with a difference due to the layer thickness measured to be 32.3%.
Optimization of the overall characteristics. In order to find an optimized set of d CPL and d MS based on quantitative evaluation, we have defined an optimization factor (γ) as where P rad and R D represent the out-coupled power to the radiation mode and the luminous reflectance. (1 -R D ) works as the CR. The definition of γ reflects the desired qualities of OLEDs for high out-coupled optical power into the radiation mode and low reflectance of the ambient light and is presented in Fig. 2b. Figure 2b shows optimization factors of MIB-OLED and conventional B-OLED in meshed surface. γ of the B-OLED does not depend on d MS (no MS layer) and is affected weakly by d CPL . Note that a circular polarizer adopted to diminish reflectance of ambient light is generally known for good performance of reducing the reflectance down to R D = 5%. However, light emission from a dipole emitter is also significantly reduced by half after a circular polarizer, i.e., the overall out-coupled power to the radiation mode falls to 50% and the luminous reflectance appears only as R D = 5% in the conventional B-OLED. With a B-OLED, γ is obtained as γ = 14.23 at d CPL = 20 nm. As the CPL is thicker, the optimization factor is decreased with a slope of Δγ/Δd CPL = − 0.023 nm −1 , i.e., for an increase of 10 nm in d CPL , γ is reduced by 1.6% with respect to the peak value. The optimization factor is finally obtained as 12.39 when d CPL = 100 nm. Because the layer thicknesses of a B-OLED are designed www.nature.com/scientificreports/ to maximize the out-coupling power at λ = 520 nm, a thicker CPL causes a change of constructive interference in the OLED cavity, thereby reduces the out-coupled power to the radiation mode. In contrast, γ of the MIB-OLED in Fig. 2b

Effect of structural parameters of MS.
To achieve further enhancement of OCE and CR, we investigate the effect of structural parameters. The length of a shorter slot L 2 and slot width W in the MS were varied, which influence SP localization. In this analysis, we have set d CPL = 40 nm and d MS = 20 nm.
Out-coupling efficiency and reflection characteristics. For simplicity, L 1 is fixed at 240 nm. L 2 and W were changed in the range of L 2 = 120-220 nm and W = 60-110 nm. In Fig. 2c, OCE reaches the minimum when W = 90 nm. The OCE of the B-OLED tends to slightly increase with longer L 2 and larger W. This is conceptually obvious because longer L 2 and larger W are directly connected with a smaller area of the absorbing metal and thus higher likelihood of light waves to transmit through MS. However, LSP has a weak effect on the emitted light from the dipole emitter, therefore the OCE depends only weakly on L 2 and W. On the other hand, structural parameters have a more visible effect on the reflectance of the ambient light. With L 2 = 210 nm, the minimum reflectance was obtained as 26.1% in the case of W = 70 nm. As L 2 becomes longer, W corresponding to the minimum reflectance decreases, i.e., LSP is well excited from the appropriate balance of the slot structure. In the case of long L 2 and large W, the reflectance dramatically increases up to 46.4% at L 2 = 220 nm and W = 110 nm. The large area of the slot structure tends to suppress excitation of LSP and causes reflectance of the ambient light to be high.
Optimization of the overall characteristics. The optimization factor γ between B-OLED and MIB-OLED is described in Fig. 2d. The flat surface in gray presents the optimization factor of the B-OLED at d CPL = 40 nm. The optimization factor of a B-OLED was obtained as 13.81 regardless of the parameters with no mixed-slot structure. In contrast, the optimization factor of a MIB-OLED is much higher than that of B-OLED for the majority of the combinations of L 2 and W, mostly for those with L 2 < 190 nm and W < 100 nm. The maximum was achieved as γ max = 16.02 when L 2 = 220 nm and W = 60 nm, i.e. the enhancement associated with MS reaches 16% (= 16.02/13.81), compared to the conventional B-OLED. These structural parameters produce an OCE of 15.6% and reflectance at 26.9% and the OCE shows enhancement by 51% (= 15.6/10.3). The enhancement achieved by optimization of MS can be better understood from spatial distribution of power flow shown in Fig. 2e-h. The distribution in the cross-section (zx plane) shows that sub-optimal thick MS in Fig. 2e [green star symbol in Fig. 2a] absorbs light emission and decreases OCE to 6.03%. In contrast, Figure 2f presents the power flow with optimal MS corresponding to the case of red star symbol in Fig. 2c, in which light emitted from a dipole is efficiently coupled to MS without significant absorption and thus improves the OCE. The power distribution in the horizontal (xy) plane for external light incidence at λ = 550 nm is shown in Fig. 2g,h. In Fig. 2g with sub-optimal MS which corresponds to blue star symbol in Fig. 2a, we observe extremely weak light localization, which causes coupling of light to the cavity to be difficult and thereby reflectance to increase. On the other hand, we can clearly see efficient localization of light using optimum MS in Fig. 2h [red star symbol in Fig. 2c], which tends to reduce reflectance. Enhanced emission of light in OLED connected with efficient plasmonic localization is in good agreement with experimental data 67,68 .
One may wonder about the performance on flexible substrates such as polyimide (n = 1.75). When the MIB-OLED corresponding to red star symbol in Fig. 2c has the substrate replaced with polyimide, OCE was improved to 17.8%. This is because an increase of substrate index reduces index mismatch between substrate and organic layers. This causes light to be trapped less in organic layers under total internal reflection and results in higher OCE. On the other hand, reflectance increases slightly to 28.5% on polyimide substrate. Flexible substrates may also have finite surface curvature, which indices more diffusive emission with larger etendue. Because SPP excitation and LSP absorption spectrum on a curved surface tend to broaden at the expense of poorer contrast 69 , it may be presumed that OCE would improve with an increase of reflectance on flexible substrates for a range of surface curvature.
While the enhancement in itself represents significant performance improvement of a MIB-OLED, we emphasize that the optimization was not performed in the full parameter space to save computation resource and shorten the calculation time. Therefore, we expect further enhancement to be made with more efficient optimization algorithms based, for example, on machine learning techniques to scan the complete parameters spaces.
Angular distribution characteristics. Angular emission distribution of MIB-OLED is calculated comparing to one of conventional planar B-OLED. We choose the MIB-OLED which has optimized structural parameters corresponding to the case of red star symbol in Fig. 2c. Angular emission distribution is obtained by combining means of FEM which calculates power flow on the top surface of glass substrate with analytical method which considers the multiple reflection within glass substrate and angle conversion from glass substrate to ambient region. Reliability of combined FEM with analytical method is validated by the calculated result of angular emission distribution of planar B-OLED using generalized Fabry-Pérot model 52 . We can also define a viewing angle as the angle position where the intensity of MIB-OLED and B-OLED reaches the half of the respective maximum intensity. When compared with the standard Lambertian emission distribution as shown in Fig. 3f, MIB-OLED shows stronger forward directional emission with a viewing angle of 101° which is narrower than 122° of planar B-OLED. As a result, out-coupled emission of MIB-OLED much better approximates the emission from a Lambertian plane light source which is desired for light emitting source.
On the other hand, Figure 3g-l show spatial power distribution of MIB-OLED and planar B-OLED in the zx plane with respect to dipole orientations when time-averaged Poynting vectors represented by red arrows are placed on the top surface of a glass substrate. Despite equivalent internal radiation patterns that originate from Hertz dipole emitters, MIB-OLED shows narrower out-coupled angular emission characteristics than that of planar B-OLED, especially in cases of horizontally-aligned dipole emitters.
The results of Figs. 2, 3 suggest that MIB-OLED should exhibit stronger emission intensity while its angular emission distribution mimics that of a Lambertian source better than conventional planar B-OLED.

Experimental confirmation.
For experimental confirmation of the MIB-OLED model, we have fabricated a cavity structure integrated with MS and performed passive characterization of the structure. For a long time, many studies of nanostructure-integrated OLEDs have been conducted, where highly enhanced OCE of OLEDs has been experimentally validated [70][71][72][73] . In the case of ambient light reflection, however, high-contrast www.nature.com/scientificreports/ OLEDs have been proposed largely in conjunction with thin-film structures such as anti-reflection coating or black cathodes without any nanostructures [17][18][19][20][21][22][23][24] . For this reason, we have focused on experimental confirmation of reflection characteristics of ambient light to MS-integrated cavity structure. Organic materials of MIB-OLED such as Alq 3 , PEDOT:PSS, and TAPC are replaced with inorganic materials which have similar refractive indices for efficient and stable fabrication. Although passive characterization of the structure without complex fabrication processes does not provide a complete picture, it can still confirm the enhanced performance due to MS in the cavity. The fabrication was largely based on electron beam lithography to define the nanoscopic size of the MS structures. The schematic illustration for the fabrication procedure is presented in Fig. 4a. MS used for experimental confirmation started with sonication of a BK7 glass substrate with acetone, IPA, and water for 5 minutes. A combined layer of adhesion promoter (AR 300-80) and E-beam resist (AR-N 7520.073) was spin-coated for 1 minute at 4000 rpm. A conductive protective layer (AR-PC 5091.02) was then spin-coated with 3000 rpm. In the patterning process, a periodic slot array was exposed with an electron beam in an area of 200 μm × 200 μm. This is followed by thermal deposition of a 20-nm thick Au thin film and a 2-nm Cr adhesion layer. The sample was immersed in the remover (AR 300-70) for 1 hour on a 150 °C hot plate to lift off the sacrificing resist pattern. The fabrication steps are illustrated in Fig. 4a. The final length of the experimentally fabricated two slots were L 1 = 200 nm, L 2 = 160 nm and W = 60 nm, as shown in Fig. 4b. After fabrication of the MS layer in gold, other materials were sequentially deposited for the MIB-OLED. The CPL and EML were replaced by Al 2 O 3 , and HIL by SiO 2 . SEM images of a fabricated MS sample are shown in Fig. 4b. More details of the depth profile can be provided by image analysis with improved clarity, i.e., after gray tones corresponding to the zero height were found, measured gray values can be converted into the depth scale, as shown in Fig. 4c, which confirms that the slots are indeed 20 nm thick.
To confirm large absorption achieved with MS, an optical set-up was constructed as shown in Fig. 4d. The set-up consists of a white-light lamp (FL-1039 Xenon arc lamp, Horiba, Japan) as light source and a spectrometer (HR4000, Ocean Optics, U.S.A.) with collimation optics. L1, L2, and L3 describe a collimating light illuminator (BX-RLA2, Olympus, Japan). L4 is a tube lens with f = 100 mm. An objective lens (UMPlanFl 100X NA0.9, Olympus) was used to illuminate and acquire reflected light from a MS sample. Firstly, reflectance spectra of MS were compared to that of gold thin film, both of which were formed on the BK7 substrate. The thickness of MS and gold thin film was fixed at 20 nm while structural parameters of mixed-slot arrays for the fabrication were L 1 = 200 nm, L 2 = 160 nm, and W = 60 nm. Incident light was unpolarized and normal to the MS and the gold thin film. Figure 4e shows an experimental reflectance spectrum of a MS sample (red solid line with symbols of filled circles) which is 1.9-fold lower on average than the reflectance of gold thin film (black solid line with symbols of open triangles) in the 450 to 650 nm visible wavelength range. These results are overall in good agreement with the calculated reflectance spectra, as shown in Fig. 4e (dashed lines in red and black). The discrepancy between experimental and numerical data appears to arise from the imperfection in the fabricated slot array size and shape of MS, which may have caused a shift in the wavelength at which LSP is induced. Nonetheless, the result confirms that MS produces large absorption of light, causing the excitation of LSP, which shows up as reduced reflectance.
The reflection of ambient light by the MS-integrated cavity structure was also measured in an identical setup. Figure 4f shows the measured and simulated reflectance spectra in the 450 to 650 nm visible wavelength range. Measured results (red solid line with circular symbols) agree well with the simulation (dashed line in red). We have also compared the reflectance spectrum between conventional B-OLED (dashed in black) and MSintegrated cavity structure (dashed in red). Note that conventional B-OLED shows strong reflection (above 80%) due to the aluminum cathode in the whole visible wavelength range. By comparison, the MS-integrated cavity structure presents significantly lower reflection with high possibility to reduce luminous reflectance, especially in the range of 525 to 575 nm wavelength where eye sensitivity can be strongly associated. The reduced reflectance in the wavelength range 500-575 nm is associated with absorption by excited SPPs that arise from the coupling between Al electrode and gold nanoslot layer. The reflectance in the longer waveband may also be affected due to absorption by LSP excitation. It was found that the effect of SPPs is less affected by the nanoslot width than that of LSPs, i.e., the absorption peaks due to LSPs tend to be blue-shifted as the nanoslots become wider. The minimum reflectance was obtained as 13.8% at 529 nm (experiment) and 12.5% at 535 nm (simulation). This represents reduction of reflectance by about 5.9 and 6.5 times, respectively, in reference to 81.7% at 530 nm for conventional B-OLED. These results suggest that MIB-OLED can improve the optical performance significantly.
We now discuss changes in the electrical properties of OLEDs caused by the introduction of a MS layer. In the MIB-OLED structure shown in Fig. 1b, because MS is separated from anode by the capping layer (TAPC) and is not in direct contact with anode, electron-hole pair recombination is affected little by the MS and its effect on electric properties such as hole carrier mobility is weak. In other words, LSP absorption that is associated with reduced back reflection due to the MS tends not to influence carrier mobility significantly, though this may increase injected current density. Such as trend is overall confirmed in other studies, e.g., when SP localized by aluminum nanoparticles embedded in a HIL, hole carrier injection and transport were found not to be affected by LSP absorption 74 . Also, embedding gold nanoparticles in a HIL, while enhancing optical efficiency, did not significantly affect hole injection efficiency 75 . On the other hand, anode replaced with a metallic mesh electrode was found to decrease hole injection barrier height and thereby obtain high current density 76 . Furthermore, luminance efficiency is improved due to SP localization, for example, as a result of energy transfer between LSP and photon radiated in an EML or reduced lifetime of exciton through Purcell effect. www.nature.com/scientificreports/ www.nature.com/scientificreports/

Conclusion
In summary, we have investigated performance enhancement of B-OLEDs integrated with MS. Effect of layer thicknesses and structural parameters has been investigated to improve performance measures such as OCE and reflectance of the ambient light. Quantitative evaluation of performance was measured by an optimization factor γ. To the best of our knowledge, this is the first study to explore integration of MS to high-contrast OLED structure. Improvement was first made by optimizing d CPL and d MS : with optimization of layer thicknesses, performance of MIB-OLED was shown to enhance by merely 3.9% over conventional B-OLED with γ max = 14.35. Further improvement was made by optimizing structural parameters L 2 and W of MS. The maximum optimization factor was achieved as γ max = 16.02, i.e. the enhancement associated with MS reaches 16%, compared to the conventional B-OLED. These structural parameters produce an OCE of 15.6% and reflectance at 26.9% and the OCE shows enhancement by 51% over that of B-OLED. Angular emission distribution of optimized MIB-OLED has a more Lambertian-like pattern than that of planar B-OLED. Enhanced optical performance of MIB-OLED is validated by experimental results. With higher γ to be achieved using more efficient optimization algorithms, we expect MS to be extremely useful as an element to improve the performance of conventional OLED structures. www.nature.com/scientificreports/